Chemical/Physical Pressure Tunable Spin-Transition Temperature and Hysteresis in a Two-Step Spin Crossover Porous Coordination Framework
Jian-Bin Lin; Wei Xue; Bao-Ying Wang; Jun Tao; Wei-Xiong Zhang; Jie-Peng Zhang; Xiao-Ming Chen; Inorganic Chemistry 51 (2012) 9423–9430; doi:10.1021/ic301237p

data_4330242
_publ_section_title
;
 Chemical/Physical Pressure Tunable Spin-Transition Temperature and
 Hysteresis in a Two-Step Spin Crossover Porous Coordination Framework
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              9423
_journal_page_last               9430
_journal_paper_doi               10.1021/ic301237p
_journal_volume                  51
_journal_year                    2012
_chemical_formula_sum            'C24 H14 Br2 Fe N10'
_chemical_formula_weight         658.12
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                88.809(5)
_cell_angle_beta                 103.415(5)
_cell_angle_gamma                89.486(5)
_cell_formula_units_Z            2
_cell_length_a                   8.5092(5)
_cell_length_b                   14.6903(10)
_cell_length_c                   10.2033(6)
_cell_measurement_reflns_used    1788
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      62.4901
_cell_measurement_theta_min      3.0008
_cell_volume                     1240.25(14)
_computing_cell_refinement
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.34.44 (release 25-10-2010 CrysAlis171 .NET)
(compiled Oct 25 2010,18:11:34)
;
_computing_data_collection
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.34.44 (release 25-10-2010 CrysAlis171 .NET)
(compiled Oct 25 2010,18:11:34)
;
_computing_data_reduction
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.34.44 (release 25-10-2010 CrysAlis171 .NET)
(compiled Oct 25 2010,18:11:34)
;
_computing_molecular_graphics    'SHELXTL Ver. 6.12, (Sheldrick, 2000)'
_computing_publication_material  'SHELXTL Ver. 6.12, (Sheldrick, 2000)'
_computing_structure_refinement  'SHELXTL Ver. 6.12, (Sheldrick, 2000)'
_computing_structure_solution    'SHELXTL Ver. 6.12, (Sheldrick, 2000)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 0.988
_diffrn_measured_fraction_theta_max 0.988
_diffrn_measurement_device_type  'Xcalibur, Sapphire3, Gemini ultra'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.1382
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            7018
_diffrn_reflns_theta_full        62.65
_diffrn_reflns_theta_max         62.65
_diffrn_reflns_theta_min         3.01
_exptl_absorpt_coefficient_mu    8.949
_exptl_absorpt_correction_T_max  0.6632
_exptl_absorpt_correction_T_min  0.5346
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.34.44 (release 25-10-2010 CrysAlis171 .NET)
(compiled Oct 25 2010,18:11:34)
empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            dark-red
_exptl_crystal_density_diffrn    1.762
_exptl_crystal_description       block
_exptl_crystal_F_000             648
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.526
_refine_diff_density_min         -0.870
_refine_diff_density_rms         0.183
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.002
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     338
_refine_ls_number_reflns         7018
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.002
_refine_ls_R_factor_all          0.1012
_refine_ls_R_factor_gt           0.0636
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0600P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1575
_refine_ls_wR_factor_ref         0.1679
_reflns_number_gt                4266
_reflns_number_total             7018
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic301237p_si_002_8.cif
_cod_data_source_block           1_173K
_cod_original_cell_volume        1240.25(13)
_cod_database_code               4330242